Uploaded by email2rajdeep

# A Review of Moisture Diffusion Coefficients in Transformer Solid Insulation—Part 2

advertisement
```This is a postprint version of the following published document:
Garc&iacute;a, D. F., [et al.] (2013). A review of moisture diffusion coefficients in
transformer solid insulation - Part 2: experimental validation of the
coefficients. IEEE electrical insulation magazine, vol. 29, no. 2, pp. 40-49.
Avalaible in http://dx.doi.org/10.1109/MEI.2013.6457598
&copy; 2013 IEEE. Personal use of this material is permitted. Permission from
IEEE must be obtained for all other uses, in any current or future media,
including reprinting/republishing this material for advertising or
promotional purposes, creating new collective works, for resale or
redistribution to servers or lists, or reuse of any copyrighted component of
this work in other works.
A Review of Moisture Diffusion Coefficients in Transformer
Solid Insulation—Part 2: Experimental Validation of the
Coefficients
D. F. Garc&iacute;a, R. Villarroel, B. Garc&iacute;a, and J. C. Burgos
Keywords: transformer solid insulation, moisture, moisture dynamics, diffusion coefficient, Kraft
paper, pressboard
Introduction
Moisture dynamics in cellulosic insulation can be estimated
using a mathematical model of diffusion based on Fick’s second
law [1], [2]. The main parameter of this mathematical model is
the moisture diffusion coefficient, and the precision of the model
is dependent on using an accurate value of this coefficient.
Various researchers have obtained expressions for the moisture diffusion coefficient for cellulosic insulation, such as Kraft
paper or pressboard, applying different methodologies [3]–[10].
Several values of the diffusion coefficient can be found in the
literature represented by mathematical expressions, tables, or
experimental curves, relating the dependence of the coefficient
with the local moisture concentration and temperature. Some of
these coefficients have been determined for nonimpregnated insulation (mainly Kraft paper and pressboard) and others for oilimpregnated paper. Most of these coefficients were determined
more than 25 years ago [11], and until now, no coefficients have
been proposed for oil-impregnated pressboard.
The objective of this article is to experimentally verify the
diffusion coefficients proposed by the various researchers. To
validate these coefficients, drying experiments were carried out
on impregnated and nonimpregnated paper and on pressboard
samples. Taking into account the characteristics of the tested
samples, two different experiments were performed:
•
•
For nonimpregnated insulation, thermo-gravimetric experiments were performed determining the weight of a
sample while being dried.
For impregnated paper, drying experiments were carried out in hot oil in which samples were periodically
extracted and analyzed by the Karl Fischer method.
The drying experiments were simulated using a diffusion
model [2], solved by finite element analysis. The simulations
D. F. Garc&iacute;a
Universidad Carlos III de Madrid,
Electrical Engineering Department,
C/Butarque 15, 28911 Legan&eacute;s (Madrid),
Spain, and Universidad del Valle, School
of Electrical and Electronic Engineering,
C/13 N&ordm; 100-00, Cali, Colombia
R. Villarroel, B. Garc&iacute;a, and J. C. Burgos
Universidad Carlos III de Madrid,
Electrical Engineering Department,
C/Butarque 15, 28911 Legan&eacute;s (Madrid),
Spain
Part two of this two-part article provides experimental validation of
the moisture diffusion coefficients
for Kraft paper and pressboard insulations in transformer oil that
have been proposed by various
researchers.
1
Figure 1. TeḀon pans ἀlled with Kr aft paper or pr essboard to the r equired thickness for thermogravimetric analyzer experiments.
were carried out using the diffusion coefficients proposed by the
various researchers. Finally, the experimental results were compared with the simulated ones, and the accuracy and the range of
application of the various coefficients were determined.
Experimental
The verification of the diffusion coefficients was performed
by using the data obtained from two sets of drying experiments.
Drying processes were carried out on nonimpregnated and on
oil-impregnated insulation, and the tests were done on Kraft
paper and pressboard, at various temperatures, and for several
insulation thicknesses.
Experiments on Nonimpregnated Insulation
To validate the moisture diffusion coefficients for nonimpregnated Kraft paper and pressboard proposed by the various
researchers, drying tests were carried out using a thermo-gravimetric analyzer (TGA).
A TGA continuously monitors the weight of a sample subjected to a temperature profile selected by the user. In the case of
nonimpregnated insulation samples, the weight loss is related to
the loss of water, and thus with the rate of drying of the sample.
Thermo-gravimetric analysis has been used by several researchers [12], [13] in analyzing the drying processes in various materials, for example, food and construction materials.
In this work, thermo-gravimetric experiments were carried
out using a thermo-gravimetric analyzer TA model Q500 on
several thicknesses of Kraft paper subjected to various drying
temperatures. Additionally, these tests were repeated on pressboard samples.
Table 1. Kraft Paper and Pressboard Samples for Thermo-Gravimetric
Analyzer Tests.
Kraft paper
Pressboard
Thickness (mm)
1, 2, 3, 4
1, 2, 3
Temperature (&deg;C)
40, 50, 60, 70, 80
40, 50, 60, 70, 80, 90, 100, 120
Sample Preparation
Before beginning the TGA experiments, the samples were
prepared with high initial moisture content. To achieve uniform
moisture content, Kraft paper and pressboard samples were kept
in a climatic chamber under controlled humidity and temperature. According to the Jeffries’ curves [14], the paper samples
were moistened at 30&deg;C and at 67.5% relative air humidity for a
minimum of 48 hours. In the case of pressboard, which is characterized by a higher density, the humectation conditions were
35&deg;C and 70% relative air humidity for at least four weeks.
Before beginning the TGA tests, the initial moisture content
of the samples was determined using the Karl Fischer titration
method, obtaining values of water content around 7.5 wt %.
Multiple layers of Kraft paper, 6 mm in diameter and 0.1 mm
thick, were compressed into a Teflon pan with a single opening
at the top until the required thickness was attained (Figure 1). As
an example, to obtain a 5-mm-thick sample, 68 layers of Kraft
paper were used. The pressboard samples were also put into
these pans to ensure unidirectional diffusion during the TGA
drying experiments. The conditions applied to Kraft paper and
pressboard samples during the drying experiments are summarized in Table 1.
TGA Experiments
The pans, filled with the insulations, were introduced into the
TGA oven (Figure 2), where they were dried under controlled
temperature until full moisture desorption. The loss of mass of
the samples was continuously monitored during the drying experiments.
During the tests, dry nitrogen was circulated through the oven
to prevent oxidation of the materials and to ensure a moisturefree atmosphere. Moreover, by fixing the gas flow, rapid release
of moisture from the sample surface is achieved, making diffusion the dominant mechanism in the drying process.
The TGA experiments give plots of weight loss due to the
release of water as a function of time, from which the average
moisture as a function of time can be calculated (Figure 3).
Experiments on Oil-Impregnated Insulation
To carry out drying experiments on oil-impregnated samples,
an apparatus was constructed to achieve moisture desorption by
2
Figure 2. Illustr ation of pan ἀlled with insulation in thermogravimetric analyzer (TGA) oven.
circulating hot and dry oil. Figure 4 shows the oil circulation
drying apparatus.
Sample Preparation
Experiments were performed on insulation specimens of 1-,
3-, and 5-mm thicknesses obtained by paper sheets of Kraft paper of 0.1-mm thickness wound on an aluminum core (Figure 5).
The core is fitted with stoppers at the top and bottom limiting
moisture desorption in longitudinal direction.
Before impregnating the samples with oil, the specimens
were kept in a climatically controlled chamber at 35&deg;C and 70%
relative air humidity for a minimum of two weeks. The conditions applied during this period were established, taking into account the Jeffries’ curves [14], to obtain an equilibrium concentration close to 8%. The specimens were then submerged in oil
at room temperature and at atmospheric pressure for a minimum
of one week. Finally, the oil-impregnated test specimens were
reintroduced into the climatic chamber to rewet the insulation
prior to the drying experiments.
Drying Experiments
As mentioned above, the drying experiments consisted of
subjecting the specimens (Figure 6), previously wetted and impregnated with oil, to a constant flow of hot dry oil. Before beginning the experiments, samples were extracted from test specimens and analyzed by Karl Fischer titration to determine the
initial moisture content, which is the average moisture throughout the thickness of the samples.
Throughout the drying process, samples were carefully extracted (Figure 7) from the specimens to determine the moisture
evolution. To validate the diffusion coefficients for oil-impregnated paper, specimens of three thicknesses (1, 3, and 5 mm)
were dried by oil circulation at four temperatures (60, 70, 80,
and 85&deg;C).
Figure 3. Evolution of average moisture content from Kraft paper in (a) and pressboard in (b) at various temperatures and for
insulation thickness of 2 mm.
Simulation of Drying Experiments
Diffusion Model
To validate the coefficients proposed by the various researchers, the drying experiments were simulated by a diffusion model
based on Fick’s second law (1) using the various coefficients. As
described in part one of this article [11], the diffusion coefficient
of cellulosic insulation depends on moisture concentration, giving a nonlinear second-order differential equation. To solve this
equation, the finite element method was applied by using Comsol Multiphysics&reg;.
∂c
∂ 
∂c 
=

D ⋅
∂t
∂x 
∂x 
(1)
3
Figure 4. Oil circulation drying apparatus; general scheme in (a) and photograph in (b) showing sample container (1), oil ἀlter
(2), circulating pump (3), expansion cup (4), and heater (5).
Boundary Conditions
To define the boundary conditions in the simulations of the experiments on nonimpregnated and on oil-impregnated samples,
several assumptions were made. In both cases, impermeability,
with regard to moisture diffusion, was considered in the inner
part of the insulation, as in both experiments the insulation was
either in contact with a Teflon pan or an aluminum core. Regarding the boundary condition on the contact surface between the
insulation and the surrounding medium, equilibrium was considered. In the TGA experiments, a moisture-free atmosphere
was created by nitrogen, and thus the moisture concentration on
the surface was considered to be zero. However, in the drying
experiments using the oil circulation apparatus, the equilibrium
condition was calculated from Fessler’s approach (2)
 4725.6 
C equil = 2.173 ⋅ 10−5 ⋅ pv0.6685 ⋅ exp 
,
 T 
(2)
where Cequil is the equilibrium moisture in paper, expressed as
a percentage, and pv is the moisture partial pressure, in atmospheres, that can be calculated from oil relative humidity HR as
pv = HR ⋅ pv, sat =
ppm
⋅p ,
ppm sat v, sat
(3)
where ppm is moisture concentration in oil expressed in parts
per million and ppmsat and pv,sat are moisture concentration and
partial pressure (atm) at saturation [5]. The partial pressure of
the saturated water was obtained by the correlation proposed by
Foss in [8], and the moisture concentration for saturation can be
obtained from the following expression:
log(ppmsat) = A − B/T,
(4)
where A and B are constants adjusted to the experimental data
[5], and the values A = 7.42 and B = 1,670 have been used in
this work.
Fitting Quality Quantiἀcation
The difference between the simulated and the experimental curves was quantified by the root-mean-square deviation
(RMSD) (5) applied to the complete drying time:
RMSD =
1
n
n
∑ C exp (ti ) − C est(ti )
2
,
(5)
i =1
where n is the number of experimental measurements, Cexp is the
measured average moisture concentration, C est is the estimated
average moisture concentration, and ti is the instant of the drying
experiment when the ith measurement was performed.
4
Figure 7. Punch extraction (a) of insulation samples (b) to de termine moisture content during drying.
Figure 5. Insulation test sample details: aluminum core (1), paper insulation (2), heating element lead (3), and internal insu lation temperature sensor (4).
Results
It was shown in part one of this article [11] that several researchers obtained coefficients for paper or pressboard, while
others proposed curves or equations that can be used to simulate
moisture dynamics in transformer insulation, and a summary is
shown in Table 2. Most of the available coefficients are based
on the empirical equation (6) proposed by Guidi [5]. The experimental drying curves were compared with those obtained by
simulation using the model described, and the coefficients that
Figure 6. Insulation specimens inside the sample container.
have been proposed by the various researchers were validated.
The agreement between the curves was quantified by means of
(5).
D = DG



kc +E  1 − 1 
a 


T0 Tk 

⋅e
(6)
It must be pointed out that Howe and Asem [3], [7], [9] used
a very particular experimental method, subjecting and analyzing pressboard samples under mechanical compression during
the drying experiments. Moreover, these researchers obtained
the coefficients at a single temperature. For these reasons these
coefficients will not be validated experimentally in this article.
Nonimpregnated Pressboard
As reflected in Table 2, Du proposed to use Guidi’s equation
(6) to calculate the moisture diffusion coefficient for pressboard
[6] and determined the values of its parameters for nonimpregnated pressboard. To this aim, she performed experiments on
nonimpregnated pressboard using an interdigital dielectrometry
sensor, and the following values were obtained: DG = 2.25 &times;
10−11 m2&middot;s−1, k = 0.1955, and Ea = 8,834 K.
As described above, drying experiments were performed using TGA to validate Du’s coefficient. Pressboard samples of
several thicknesses were subjected to various temperatures until
total moisture desorption was achieved. These experiments were
simulated by finite element analysis applying Du’s coefficient
to (1), and the difference between the measured and simulated
drying curves was calculated using (5).
The RMSDs obtained for all of the simulated cases are shown
in Figure 8 and Table 3. It can be seen that the RMSDs are very
different, and as large as two orders of magnitude, depending
on temperature and sample thickness. It is observed that lower
RMSDs between measured and simulated drying curves are obtained with the experiments performed on 1-mm-thick samples.
For thicker samples, the results of Du’s coefficient are worse.
5
Table 2. Moisture Diffusion Coefficients for Transformer Insulation Proposed by Various Researchers.
Researcher
Ast
Paper
(nonimpregnated)
Paper
(impregnated)
Pressboard
(nonimpregnated)
x
Guidi
Coefficient
expression
Equation D(C,T)1
x
Howe
x2
Asem
x
x
Foss
x
x
Du
Equation D(C,T)
x
Tables and curves
x
Tables and curves
Equation D(C,T)
x
Equation D(C,T)
Equation obtained by Du from Ast’s experimental data.
Determination on Manila paper.
1
2
To grasp the significance of the RMSD, the results of two
simulations are shown in Figure 9. Figure 9(a) corresponds to a
measurement performed on a 1-mm-thick sample dried at 60&deg;C.
In this case the obtained RMSD is 1.30 &times; 10−01, and the simulated values show good agreement with the experimental ones.
On the other hand, Figure 9(b) shows the same comparison on
a 2-mm-thick sample dried at 70&deg;C. In this case the obtained
RMSD is 9.20 &times; 10−01, and the simulated values show poor
agreement with the experimental ones, with drying times estimated by Du’s coefficient being one-third of the actual times,
i.e., 500 verses 1,500 minutes.
From the analysis it can be concluded that Du’s coefficient
works well when it is applied to thin samples while the estimation of the moisture diffusion for thick samples is poor. To
Figure 8. Root-mean-squar e deviation (RMSD; dif ference be tween the simulated and e xperimental values) of Du’ s coefἀcient for nonimpregnated pressboard.
Figure 9. Simulated and measur ed moistur e diffusion coefἀcients in pressboard: (a) 1-mm thickness at 60&deg;C and (b) 2-mm
thickness at 70&deg;C.
6
Table 3. Root-Mean-Square Deviation (RMSD) Obtained by Du’s Coefficient for Nonimpregnated Pressboard.
Temperature (&deg;C)
40
50
60
70
80
90
100
120
Thickness
(mm)
Table 4. Root-Mean-Square Deviations (RMSD) Obtained by
Foss’s and Ast’s Coefficient for Nonimpregnated Paper.
RMSD
RMSD DDu
1
1.94 &times; 10−01
2
1.83 &times; 10+00
3
2.13 &times; 10+00
1
1.57 &times; 10−01
2
1.22 &times; 10+00
3
1.53 &times; 10+00
1
1.30 &times; 10−01
2
9.84 &times; 10−01
3
1.81 &times; 10+00
1
8.25 &times; 10−02
2
9.20 &times; 10−01
3
1.24 &times; 10+00
1
9.10 &times; 10−02
2
6.64 &times; 10−01
3
1.20 &times; 10+00
1
1.08 &times; 10−01
2
4.85 &times; 10−01
3
1.07 &times; 10+00
1
8.32 &times; 10−02
2
3.26 &times; 10−01
3
6.01 &times; 10−01
1
1.40 &times; 10−01
2
2.04 &times; 10−01
3
6.22 &times; 10−01
Temperature
(&deg;C)
40
50
60
70
80
Thickness
(mm)
DFoss
DAst
2
4.54 &times; 10−01
1.56&times;10−01
3
1.29 &times; 10−01
5.01&times;10−01
4
2.52 &times; 10−01
9.36 &times; 10−01
5
4.99 &times; 10−01
1.37
2
3.67 &times; 10−01
1.71 &times; 10−01
3
1.22 &times; 10−01
2.60 &times; 10−01
4
1.26 &times; 10−01
4.05 &times; 10−01
5
1.39 &times; 10−01
6.18 &times; 10−01
2
4.26 &times; 10−01
2.68 &times; 10−01
3
1.85 &times; 10−01
9.02 &times; 10−02
4
2.38 &times; 10−01
1.84 &times; 10−01
5
1.73 &times; 10−01
4.46 &times; 10−01
2
3.47 &times; 10−01
2.50 &times; 10−01
3
2.14 &times; 10−01
1.15 &times; 10−01
4
2.14 &times; 10−01
9.23 &times; 10−02
5
1.80 &times; 10−01
1.72 &times; 10−01
2
2.87 &times; 10−01
2.29 &times; 10−01
3
1.80 &times; 10−01
1.26 &times; 10−01
4
1.79 &times; 10−01
8.22 &times; 10−02
5
2.49 &times; 10−01
1.02 &times; 10−01
Nonimpregnated Kraft Paper
understand this result, it must be remarked that all the diffusion
experiments performed by Du for the determination of her coefficeint were carried out on samples of 1.5-mm thickness, and
the obtained results seem to indicate that the coefficient is valid
in the thickness range studied, whereas the obtained results are
poorer when applied to thicker insulation.
The dependence of the moisture diffusion coefficient on sample thickness has not been considered by any of the researchers
who worked on transformer insulation. However, that dependence has been described by other researchers in the determination of moisture diffusion coefficients of various hygroscopic
materials [15]–[19].
In the case of nonimpregnated Kraft paper, two different coefficients have been proposed by Foss and Ast (Table 2), and
both are based on Guidi’s equation. The values proposed for the
parameters in each case being DG Foss = 2.62 &times; 10−11 m2&middot;s−1, k Foss
= 0.5, Ea Foss = 8,140 K and DG Ast = 2.25 &times; 10−11 m2&middot;s−1, k Ast =
0.1955, Ea Ast = 8,834 K.
These coefficients are used to simulate the TGA drying experiments of Kraft paper samples dried at various temperatures
(Table 1). The RMSDs between the simulated and measured values when Foss’s or Ast’s coefficients are used are shown in Table
4 and also in Figure 10. The experimental and simulated curves
for two different cases are plotted in Figure 11. It can be seen in
Figure 10 that Foss’s coefficient is more accurate in most cases,
especially at low temperatures.
7
Figure 10. Root-mean-squar e deviation (RMSD) of F oss’s (a)
and Ast’s (b) for the moistur e dif fusion coefἀcient in nonim pregnated paper.
Figure 11. Simulated and measur ed moisture diffusion coefἀcients for nonimpr egnated paper: (a) 2-mm thic kness at 60&deg;C
and (b) 3-mm thickness at 80&deg;C.
Oil-Impregnated Kraft Paper
The moisture diffusion coefficients proposed by Foss and
Guidi were validated on samples of oil-impregnated Kraft paper
of various thicknesses and oil temperatures. The moisture content in the oil, required for the simulation of the drying process,
was measured by a moisture sensor in the drying apparatus. The
RMSDs for the diffusion coefficients (Table 5) are significantly
higher than those simulated for nonimpregnated insulation. Possible reasons for the increased RMSD include the uncertainty in
the Karl Fischer measurements and the discrete rather than continuous moisture measurements during the drying experiments.
On the other hand, the determination of the moisture diffusion
coefficient in oil-impregnated materials is complex, and the obtained expressions are less precise compared with those on nonimpregnated samples. It may also be observed that Guidi’s coefficient provides better estimates than does Foss’s coefficient.
The comparison between the measured and estimated values for two simulations is shown in Figure 12. The simulations
correspond to a 5-mm-thick sample dried in oil at 60&deg;C and a
3-mm-thick sample dried at 70&deg;C. By analyzing these two experimental cases, the precision of Foss’s and Guidi’s coefficients
can be estimated.
From the plots shown in Figure 12, the moisture level after
the drying process was about 3%, in both cases, and the time to
attain this level was nearly 25 days for the 5-mm sample at 60&deg;C
(Figure 12a) and about 20 days for the 3-mm-thick sample dried
at 70&deg;C (Figure 12b). In Figure 12a, it is observed that Guidi
predicts a realistic evolution of moisture, while Foss estimates
that 3% moisture is reached in 10 days, which is too optimistic.
In Figure 12b, the estimates using the coefficients from both researchers are unrealistic in that Guidi’s coefficient predicts that
a moisture level of 3% is attained in just over four days while
Foss’s coefficient is even more optimistic, predicting the same
level in less than two days. Similar patterns are found in the
other simulations. Guidi’s, and specially Foss’s, coefficients pre-
8
Table 5. Comparison of Root-Mean-Square Deviation (RMSD) Obtained
by Foss’s and Guidi’s Coefficient of Moisture Diffusion for Impregnated
Paper.
Temperature
(&deg;C)
60
70
80
85
RMSD
Thickness
(mm)
DFoss
DGuidi
5
1.628
0.737
1
2.260
2.046
3
3.080
2.293
5
2.462
1.465
1
3.529
3.430
3
2.612
2.083
5
1.677
0.569
1
2.178
2.094
3
2.097
1.385
5
1.708
0.585
dict a moisture desorption much too fast in most cases, although
Guidi’s coefficient works better on 5-mm-thick samples.
Conclusions
The coefficient of moisture diffusion is an important parameter in the modeling of moisture dynamics in transformer solid
insulation, and various researchers have proposed coefficients
valid for Kraft paper and pressboard insulating materials. In this
work, the proposed coefficients have been tested by means of
drying experiments performed at various temperatures.
The behavior of Du’s moisture diffusion coefficient in nonimpregnated pressboard has been tested. The coefficient works
well for 1-mm-thick samples but not for thicker samples. The
dependence of the diffusion coefficient on thickness has also
been observed in other materials, but none of the proposed coefficients for transformer insulation include that dependence.
The coefficients proposed by Foss and Ast for nonimpregnated Kraft paper were validated using the results of thermogravimetric experiments. Foss’s coefficient is more accurate in
most cases, although the behavior of both coefficients changes
for different experimental conditions. This is especially true at
low temperatures.
The coefficients proposed by Foss and Guidi for oil-impregnated paper were verified by experiments in a hot oil drying apparatus, and using these coefficients in simulations, large
differences between the experimental and estimated results are
obtained, in that the estimated diffusion times are very short in
comparison with the measured ones. In addition, Guidi’s coefficient provides more precise estimates of the diffusion times
than does Foss’s.
As a general conclusion, it appears that the available coefficients for modeling moisture dynamics in transformer insulation
are not as precise as would be desirable. Additional work needs
Figure 12. Simulated and measured coefἀcients of moisture diffusion in impregnated paper: (a) thickness of 5 mm at 60&deg;C and
(b) thickness of 3 mm at 70&deg;C.
to be done to obtain the moisture diffusion coefficient expressions as a function of thickness, temperature, and moisture concentration. Moreover, no coefficient is available to calculate the
moisture diffusion in oil-impregnated pressboard, and the need
for this great, as this part of transformer insulation retains the
larger percentage of moisture.
Acknowledgments
This work was financed by the Spanish Ministry of Science and Technology under the project DPI2009-07093. Diego
F. Garc&iacute;a is an assistant professor at the Universidad del Valle
(Colombia) and is currently on leave at the Universidad Carlos
III de Madrid, Spain. The pressboard samples used in this work
were provided by the transformer manufacturer Cotradis (Grupo
Ormazabal).
9
References
[1]
[2]
[3]
[4]
[5]
[6]
[7]
[8]
[9]
[10]
[11]
[12]
[13]
[14]
[15]
[16]
[17]
[18]
[19]
J. A. Almendros-Iba&ntilde;ez, J. C. Burgos, and B. Garcia, “Transformer field
drying procedures: A theoretical analysis,” IEEE Trans. Power Del., vol.
24, no. 4, pp. 1978–1986, Oct. 2009.
D. F. Garc&iacute;a, B. Garc&iacute;a, and J. C. Burgos, “Modeling power transformer
field drying processes,” Drying Technol., vol. 29, no. 8, pp. 896–909,
May 2011.
F. Howe, “The diffusion of moisture through power transformer insulation,” PhD dissertation, Dept. Electr. Electron. Eng., Univ. Nottingham,
UK, 1975.
P. F. Ast, “Movement of moisture through A50P281 Kraft paper (dry
and oil impregnated),” General Electric, Tech. Rep. Test Report, HVER-66-41, 1966.
W. Guidi and H. Fullerton, “Mathematical methods for prediction of
moisture take-up and removal in large power transformers,” in Proceedings of Winter Meeting of IEEE Power Engineering Society, C-74, 1974,
pp. 242–244.
Y. Du, “Measurements and modeling of moisture diffusion processes in
transformer insulation using interdigital dielectrometry sensors,” PhD
dissertation, Dept. Electr. Eng. Comp. Sci., Massachusetts Inst. Tech.,
Cambridge, MA, 1999.
S. Asem and A. F. Howe, “Drying of power-transformer insulation,” in
IEE Proceedings Generation, Transmission and Distribution [See also
IEE Proceedings—Generation, Transmission and Distribution], vol. 129,
no. 5, pp. 228–232, Sep. 1982.
S. D. Foss and L. Savio, “Mathematical and experimental analysis of the
field drying of power transformer insulation,” IEEE Trans. Power Del.,
vol. 8, no. 4, pp. 1820–1828, Oct. 1993.
S. Asem, “The drying of power transformer insulation,” MS thesis, Dept.
Electr. Electron. Eng., Univ. Nottingham, UK, 1981.
S. D. Foss, “Power transformer drying model,” Report prepared for General Electric Company, Large Transformer Operation, Pittsfield, MA, and
Consolidated Edison Corporation, New York, NY, by Dynamic Systems,
Pittsfield, MA, 1987, pp. 16–19.
D. F. Garc&iacute;a, B. Garc&iacute;a, and J. C. Burgos, “A review of moisture diffusion
coefficients in transformer solid insulation—Part 1: Coefficients for paper
and pressboard,” IEEE Electr. Insul. Mag., vol. 29, no. 1, pp. 46–54,
2013.
S. Park, H. N. Shin, D. H. Lee, D. J. Kim, J. H. Kim, Y. K. Lee, S. J. Sim,
and K. B. Choi, “Drying characteristics of particles using thermogravimetric analyzer,” Korean J. Chem. Eng., vol. 20, no. 6, pp. 1170–1175,
Nov. 2003.
Z. Li and N. Kobayashi, “Determination of moisture diffusivity by
thermo-gravimetric analysis under non-isothermal condition,” Drying
Technol. 2005, vol. 23, no. 6, pp. 1331–1342, Jun. 2005.
R. Jeffries, “The sorption of water by cellulose and eight other textile
polymers,” Textile Inst. J., vol. 51, no. 9, pp. 339–374, Sep. 1960.
W. Fernando, H. Low, and A. Ahmad, “Dependence of the effective diffusion coefficient of moisture with thickness and temperature in convective drying of sliced materials. A study on slices of banana, cassava and
pumpkin,” J. Food Eng., vol. 102, no. 4, pp. 310–316, Feb. 2011.
P. T. Johnson, J. G. Brennan, and F. Y. Addo-Yobo, “Air-drying characteristics of plantain (musa AAB),” J. Food Eng., vol. 37, no. 2, pp. 233–242,
Aug. 1998.
Maskan, S. Kaya, and M. Maskan, “Hot air and sun drying of grape
leather (pestil),” J. Food Eng., vol. 54, no. 1, pp. 81–88, Aug. 2002.
M. Nguyen and W. E. Price, “Air-drying of banana: Influence of experimental parameters, slab thickness, banana maturity and harvesting
season,” J. Food Eng., vol. 79, no. 1, pp. 200–207, Mar. 2007.
M. A. Tutuncu and T. P. Labuza, “Effect of geometry on the effective
moisture transfer diffusion coefficient,” J. Food Eng., vol. 30, no. 3-4, pp.
433–447, Dec. 1996.
Diego F. Garc&iacute;a received his BS and MSc
degrees in electrical engineering from the
Universidad del Valle, Colombia, in 1999
and 2003, respectively, and in 2012, the
PhD degree in electrical engineering from
the Universidad Carlos III de Madrid. He
joined the School of Electrical and Electronic Engineering at Universidad del Valle
in 2001 and is now an assistant professor.
His research involves moisture dynamics and drying out of power transformers.
Rafael Villarroel was born in May 1982.
He received the MSc degree in electrical
engineering from Universidad Carlos III de
Madrid in 2012 and is currently enrolled
in the PhD program on electrical engineering at Universidad Carlos III de Madrid, in
Spain. His research is based on moisture
dynamics modeling in transformer solid
insulation.
Bel&eacute;n Garc&iacute;a received the MSc degree in
physics from Universidad Complutense de
Madrid in 1998 and the PhD degree in electrical engineering from Universidad Carlos
III de Madrid in 2002. Since 2004 she has
held an associate professor position in the
electrical engineering department of the
same university. Her main research interest
is power transformer life management.
Juan Carlos Burgos was born in 1955. He
received the PhD degree from the Escuela
T&eacute;cnica Superior de Ingenieros Industriales de Madrid in 1987. Currently, he is
an associate professor with the Universidad Carlos III de Madrid, Madrid, Spain,
where he has worked since 1994. His main
research interest is power transformer
maintenance.
10
```